Stainless Steel 304B Material Property Data Sheet
Do you need custom fasteners created with Stainless Steel 304B? Since our inception, Vegas Fastener Manufacturing has met every challenge of providing
Quality, Timely, Cost-effective solutions for specialty fastener applications. Every product is built to your specifications, using your prints if necessary.
Below are the technical specifications of the Stainless Steel 304B Bar Stock we have available to meet your needs.
Industeel NUCL 18.10 B4 Natural Boron (Min 1% wt) Alloyed 304 Stainless Steel
Subcategory: Metal; Stainless Steel; T 300 Series Stainless Steel
Key Words: aisi304, aisi 304, DIN W.14306 Bor-01 Ind.00, ASTM A887 UNS S30464 : Type 304B4, SUS304, SS304
|Component|| Wt. %|
|Fe||66.687 - 66.787|| |
|N ||Max 0.1|| |
Description: Isotope B10 has the property to capture neutrons produced by nuclear reactions. Natural boron contains about 19.9 at% or 18.45 wt % of B10 isotope, the remaining being B11 isotope. NUCL 18.10 B4 grade is a 304 stainless steel obtained by ingot casting and alloyed with 1 to 1,24 wt% natural boron additions. In order to avoid ferrite grain which reduce the ductility of the alloy, NUCL 18.10 B4 grade has been overalloyed in Nickel when compared to 304 grades. Molybdenum additions are sometimes considered to increase the corrosion resistance properties. The ingots rolled into plates are considered for nuclear applications (transport, casks, storage -in pools) of nuclear (waste) products. For specific purposes, some other grades are sometimes used. The boron content may thus be included in the 0.2-2 weight % range or/and alloys obtained by powder metallurgy (A type). CLI-FAFER can also produce 18-10 A or B type boron alloyed grades (included B10 enriched grades). Among the family of boron enriched 304 grades, NUCL 18-10 B4 grade is the most commonly used.
Iron content calculated as remainder.
Information provided by manufacturer.
|Density||7.8 g/cc||0.282 lb/in³|| |
|Hardness, Brinell||Max 217||Max 217|| Typical|
|Hardness, Rockwell B||Max 95||Max 95|| Typical|
|Tensile Strength, Ultimate||Min 515 MPa||Min 74700 psi|| Minimum Guaranteed|
|Tensile Strength, Ultimate||610 MPa||88500 psi|| Typical|
|Tensile Strength, Yield||Min 225 MPa||Min 32600 psi|| Y.S. 1%|
|Tensile Strength, Yield||Min 210 MPa||Min 30500 psi|| Y.S. 0.2%|
|Tensile Strength, Yield||310 MPa||45000 psi|| Typical (Y.S. 0.2%)|
|Tensile Strength, Yield||325 MPa||47100 psi|| Typical (Y.S. 1%)|
|Elongation at Yield||Min 16 %||Min 16 %|| |
|Elongation at Yield||19 %||19 %|| Typical|
|Modulus of Elasticity||200 GPa||29000 ksi|| 20°C|
|Poisson's Ratio||0.333||0.333|| Calculated|
|Shear Modulus||75 GPa||10900 ksi|| 20°C|
|Electrical Resistivity||9.5e-005 ohm-cm||9.5e-005 ohm-cm|| 20°C|
|CTE, linear 20°C||17 µm/m-°C||9.44 µin/in-°F|| 20-100°C|
|CTE, linear 100°C||17.5 µm/m-°C||9.72 µin/in-°F|| 20-200°C|
|CTE, linear 250°C||18 µm/m-°C||10 µin/in-°F|| 20-300°C|
|Heat Capacity||0.5 J/g-°C||0.12 BTU/lb-°F|| 20°C|
|Thermal Conductivity||15 W/m-K||104 BTU-in/hr-ft²-°F|| 20°C||
This information is provided by
MatWeb.com, The Online Materials Database and is reprinted with their permission.
Copyright 1996-2005 by Automation Creations, Inc.
The contents, results, and technical data on this page may not
be reproduced either electronically, photographically or substantively without permission from
Automation Creations, Inc and MatWeb.com. No warranty, neither expressed nor implied, is given
regarding the accuracy of this information. The user assumes all risk and liability in connection with the use of
information from MatWeb.com.